The EBR-II X501 Minor Actinide Burning Experiment Page: 7 of 11
This article is part of the collection entitled: Office of Scientific & Technical Information Technical Reports and was provided to Digital Library by the UNT Libraries Government Documents Department.
The following text was automatically extracted from the image on this page using optical character recognition software:
HW HW .HW
Table 2. Attributes of X51 minor actinide bearing fuel elements
Composition (average analyzed U-20.2Pu-9. 1Zr-i .2Am- 1.3Np
Major impurities (average wto) Si:O.26, Al:O.089, Ca:O.067,
Cr:0.0025, Mg:0.009, Fe:0.001,
U-235 enrichment (nominal) 60%o
Fuel mass 77.5 g
Fuel length 34.3 cm (13.5 in.)
Element length (nominal) 74.9 cm (29.5 in.)
Cladding type HT-9 steel
Cladding OD 5.84 mm (0.230 in.)
Cladding wall 0.457 mm (0.0 18 in.)
Slug diameter 4.27 mm (0.168 in.)
Plenum volume 7.1 cm3
Plenum gas 75He-Ar
Smeared density 750%
Fuel slug density, 99.5%o
XSO1 Postirradiation Examination
A partial postirradiation examination was completed on X50 1, including gamma scanning, optical
microscopy, microprobe analysis, and metallography. The post irradiation examination completed
Here’s what’s next.
This article can be searched. Note: Results may vary based on the legibility of text within the document.
Tools / Downloads
Get a copy of this page or view the extracted text.
Citing and Sharing
Basic information for referencing this web page. We also provide extended guidance on usage rights, references, copying or embedding.
Reference the current page of this Article.
Carmack, Jon; Hayes, S. L.; Meyer, M. K. & Tsai, H. The EBR-II X501 Minor Actinide Burning Experiment, article, June 1, 2008; [Idaho Falls, Idaho]. (digital.library.unt.edu/ark:/67531/metadc893878/m1/7/: accessed December 11, 2018), University of North Texas Libraries, Digital Library, digital.library.unt.edu; crediting UNT Libraries Government Documents Department.